#------------------------------------------------------------------------------
#$Date: 2016-02-16 03:10:39 +0200 (Tue, 16 Feb 2016) $
#$Revision: 176453 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/65/7216551.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7216551
loop_
_publ_author_name
'Gao, Qiao'
'Li, Fengyan'
'Sun, Minghui'
'Xu, Lin'
'Wang, Yuchao'
'Bai, Jie'
_publ_section_title
;
 Multidimensional all-inorganic frameworks based on new molybdovanadate
 cluster of [VMo7O28]9−with Cu(ii) linker showing semiconducting
 behavior
;
_journal_issue                   33
_journal_name_full               CrystEngComm
_journal_page_first              7681
_journal_paper_doi               10.1039/C4CE00831F
_journal_volume                  16
_journal_year                    2014
_chemical_formula_sum            'Cu8 H152 Mo30 N20 O169 V10'
_chemical_formula_weight         7033.34
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2014-05-19 # Formatted by publCIF
;
_cell_angle_alpha                96.789(2)
_cell_angle_beta                 98.188(2)
_cell_angle_gamma                93.537(2)
_cell_formula_units_Z            1
_cell_length_a                   14.7333(3)
_cell_length_b                   17.2359(6)
_cell_length_c                   18.2871(4)
_cell_measurement_reflns_used    10438
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      29.2075
_cell_measurement_theta_min      2.7668
_cell_volume                     4549.7(2)
_computing_cell_refinement       'Bruker FRAMBO'
_computing_data_collection       'Bruker FRAMBO'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.992
_diffrn_measured_fraction_theta_max 0.992
_diffrn_measurement_device_type  'multiwire proportional'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0306
_diffrn_reflns_av_unetI/netI     0.0536
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -20
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            29450
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         2.77
_exptl_absorpt_coefficient_mu    3.504
_exptl_absorpt_correction_T_max  0.704
_exptl_absorpt_correction_T_min  0.538
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    2.567
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             3366
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.15
_exptl_crystal_size_min          0.1
_platon_squeeze_details
;
;
_refine_diff_density_max         1.966
_refine_diff_density_min         -1.954
_refine_diff_density_rms         0.177
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.053
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1075
_refine_ls_number_reflns         15926
_refine_ls_number_restraints     36
_refine_ls_restrained_S_all      1.057
_refine_ls_R_factor_all          0.0636
_refine_ls_R_factor_gt           0.0453
_refine_ls_shift/su_max          0.049
_refine_ls_shift/su_mean         0.002
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0751P)²+1.7912P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1245
_refine_ls_wR_factor_ref         0.1350
_reflns_number_gt                12382
_reflns_number_total             15926
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c4ce00831f2.cif
_cod_data_source_block           p-1
_cod_depositor_comments
'Adding full bibliography for 7216550--7216552.cif.'
_cod_original_formula_sum        'H152 Cu8 Mo30 N20 O169 V10'
_cod_database_code               7216551
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
O1 O 0.5565(3) 0.8957(3) 0.8159(3) 0.0277(12) Uani 1 1 d .
O2 O 0.4387(4) 0.8371(3) 0.7043(3) 0.0337(13) Uani 1 1 d .
O3 O 0.4846(4) 0.9729(3) 0.6843(3) 0.0310(12) Uani 1 1 d .
O4 O 0.4797(4) 0.7428(3) 0.8213(3) 0.0397(14) Uani 1 1 d .
O5 O 0.3612(3) 0.8588(3) 1.0433(3) 0.0313(12) Uani 1 1 d .
O6 O 0.4519(3) 0.8656(3) 0.9198(3) 0.0306(12) Uani 1 1 d .
O7 O 0.5610(3) 1.2151(3) 0.8390(3) 0.0286(12) Uani 1 1 d .
O8 O 0.5577(3) 1.0544(3) 0.8226(3) 0.0232(11) Uani 1 1 d .
O9 O 0.3873(3) 1.1150(3) 0.8272(3) 0.0296(12) Uani 1 1 d .
O10 O 0.2084(3) 1.0035(3) 0.7829(3) 0.0325(12) Uani 1 1 d .
O11 O 0.4531(3) 1.0308(3) 0.9370(3) 0.0274(12) Uani 1 1 d .
O12 O 0.3843(3) 0.9519(3) 0.7976(3) 0.0242(11) Uani 1 1 d .
O14 O 0.6436(3) 0.9756(3) 0.9463(3) 0.0289(12) Uani 1 1 d .
O15 O 0.4840(4) 1.3053(3) 0.7301(3) 0.0393(14) Uani 1 1 d .
O16 O 0.3795(3) 1.4206(3) 0.7867(3) 0.0325(12) Uani 1 1 d .
O17 O 0.4021(3) 1.3921(3) 0.6228(3) 0.0307(12) Uani 1 1 d .
O18 O 0.2793(3) 1.4097(3) 0.5190(3) 0.0289(12) Uani 1 1 d .
O20 O 0.0673(3) 1.1840(3) 0.5557(3) 0.0298(12) Uani 1 1 d .
O21 O 0.0414(3) 1.2101(3) 0.7198(3) 0.0305(12) Uani 1 1 d .
O22 O 0.2308(4) 1.4602(3) 0.8244(3) 0.0399(14) Uani 1 1 d .
O23 O 0.1892(3) 1.1696(3) 0.8091(3) 0.0304(12) Uani 1 1 d .
O24 O 0.2326(3) 1.4401(3) 0.6676(3) 0.0301(12) Uani 1 1 d .
O25 O 0.2158(3) 1.3087(3) 0.7469(3) 0.0305(12) Uani 1 1 d .
O26 O 0.3737(4) 1.2867(3) 0.8484(3) 0.0376(13) Uani 1 1 d .
O27 O 0.4083(3) 1.2371(3) 0.5739(3) 0.0300(12) Uani 1 1 d .
O28 O 0.2421(4) 1.5588(3) 0.5753(3) 0.0397(14) Uani 1 1 d .
O29 O 0.7332(3) 1.0617(3) 0.8602(3) 0.0338(13) Uani 1 1 d .
O30 O 0.3165(4) 0.8126(3) 0.8043(3) 0.0353(13) Uani 1 1 d .
O31 O 0.1322(4) 1.0883(3) 0.6604(3) 0.0371(13) Uani 1 1 d .
O32 O 0.2361(3) 1.1318(3) 0.5428(3) 0.0317(12) Uani 1 1 d .
O33 O 0.2618(3) 1.2564(3) 0.4647(3) 0.0319(12) Uani 1 1 d .
O34 O 0.7523(4) 0.9019(4) 0.8545(3) 0.0440(15) Uani 1 1 d .
O35 O 0.2669(4) 0.9277(3) 0.9037(3) 0.0375(13) Uani 1 1 d .
O36 O 0.6508(4) 0.9640(3) 0.7317(3) 0.0327(13) Uani 1 1 d .
O37 O 0.0708(3) 1.3388(3) 0.6359(3) 0.0318(12) Uani 1 1 d .
O38 O 0.2358(3) 1.2883(3) 0.5995(3) 0.0309(12) Uani 1 1 d .
O39 O 0.4155(4) 1.5344(4) 0.5539(3) 0.0418(14) Uani 1 1 d .
O40 O -0.0772(3) 1.2518(3) 0.6062(3) 0.0368(13) Uani 1 1 d .
O41 O 0.2011(4) 1.3230(3) 0.8847(3) 0.0367(13) Uani 1 1 d .
O42 O 0.0906(3) 1.2912(3) 0.4809(3) 0.0310(12) Uani 1 1 d .
O43 O 0.0458(3) 1.3426(3) 0.7884(3) 0.0368(14) Uani 1 1 d .
O44 O 0.0495(4) 1.2211(4) 0.8760(3) 0.0497(16) Uani 1 1 d .
O45 O 0.6664(4) 1.1308(3) 0.7525(3) 0.0345(13) Uani 1 1 d .
O46 O 0.7496(4) 1.2283(4) 0.8822(4) 0.0474(16) Uani 1 1 d .
O47 O 0.5512(4) 1.4500(4) 0.7348(3) 0.0426(15) Uani 1 1 d .
O48 O 0.3578(5) 1.4183(4) 0.9393(3) 0.0551(17) Uani 1 1 d .
O49 O 0.3751(4) 1.5344(3) 0.6964(3) 0.0365(13) Uani 1 1 d .
O50 O -0.0579(4) 1.3706(3) 0.5151(3) 0.0420(14) Uani 1 1 d .
O51 O -0.0846(4) 1.4003(4) 0.6890(3) 0.0452(15) Uani 1 1 d .
O52 O 0.4328(4) 1.3373(4) 0.4770(3) 0.0421(15) Uani 1 1 d .
O53 O 0.1212(4) 1.1393(4) 0.4180(3) 0.0429(14) Uani 1 1 d .
O54 O 0.3167(4) 1.0255(3) 0.6654(3) 0.0364(13) Uani 1 1 d .
O55 O 0.4876(4) 1.1287(3) 0.6891(3) 0.0367(13) Uani 1 1 d .
O56 O -0.0900(4) 1.2203(4) 0.4540(3) 0.0461(15) Uani 1 1 d .
O57 O -0.0455(4) 1.0768(4) 0.6208(3) 0.0460(15) Uani 1 1 d .
O58 O -0.1308(4) 1.2674(4) 0.7441(4) 0.0493(16) Uani 1 1 d .
O59 O 0.3699(5) 1.5817(4) 0.8450(3) 0.0534(17) Uani 1 1 d .
O60 O 0.2156(4) 1.5887(4) 0.7467(4) 0.0524(17) Uani 1 1 d .
O61 O 0.4086(5) 1.0665(4) 0.5303(3) 0.0589(18) Uani 1 1 d .
O62 O 0.1334(4) 0.8559(4) 0.7933(4) 0.0581(18) Uani 1 1 d .
O63 O 0.6250(5) 0.7946(4) 0.7186(3) 0.0520(17) Uani 1 1 d .
O64 O 0.3478(5) 0.8943(4) 0.5722(3) 0.0561(18) Uani 1 1 d .
O65 O 0.6097(4) 1.0544(3) 0.6098(3) 0.0429(15) Uani 1 1 d .
O66 O 0.2566(4) 0.8804(3) 0.6928(3) 0.0404(14) Uani 1 1 d .
O67 O 0.5627(5) 0.8622(4) 0.5996(3) 0.061(2) Uani 1 1 d .
O68 O 0.3231(3) 1.1812(3) 0.7044(3) 0.0216(10) Uani 1 1 d .
O69 O 0.1087(6) 1.4458(6) 0.4600(7) 0.058(3) Uani 0.64 1 d PU
O70 O 0.1800(10) 1.3669(9) 0.3707(8) 0.033(3) Uani 0.36 1 d PU
O71 O 0.0814(14) 1.4631(13) 0.9135(12) 0.072(6) Uani 0.36 1 d PU
O72 O 0.0533(9) 1.5096(9) 0.8072(14) 0.145(9) Uani 0.64 1 d P
N2 N 0.6867(7) 0.3225(7) 0.7427(7) 0.095(3) Uani 1 1 d U
N4 N 0.3859(7) 0.4808(7) 0.3931(5) 0.080(3) Uani 1 1 d U
N5 N 0.9345(6) 0.0740(5) 0.3641(5) 0.065(3) Uani 1 1 d .
N6 N 0.7493(7) 0.4061(7) 0.5797(6) 0.090(3) Uani 1 1 d U
N7 N 0.6126(6) 0.2492(6) 0.5931(7) 0.093(4) Uani 1 1 d .
N8 N 0.7930(7) 0.9927(7) 0.6532(7) 0.097(4) Uani 1 1 d .
N9 N 0.0315(7) 0.0289(8) 0.8290(8) 0.110(4) Uani 1 1 d .
O2W O 0.5464(8) 0.6272(6) 0.7199(9) 0.153(6) Uani 1 1 d .
N1 N 0.8789(5) 0.1065(5) 0.7796(5) 0.057(2) Uani 1 1 d .
N10 N 0.7619(5) 0.1482(6) 0.5753(5) 0.069(3) Uani 1 1 d .
O1W O 0.8453(5) 0.0302(4) 0.4837(4) 0.071(2) Uani 1 1 d .
O3W O 0.0549(5) 0.5116(5) 0.6146(5) 0.074(2) Uani 1 1 d .
O6W O 0.2713(12) 0.7285(8) 0.9284(7) 0.076(5) Uani 0.50 1 d P
O8W O 0.5933(13) 1.3790(11) 0.9098(12) 0.117(8) Uani 0.50 1 d P
O9W O 0.5391(13) 1.5249(13) 0.9084(11) 0.120(8) Uani 0.50 1 d P
O10W O 0.2466(15) 0.5813(13) 0.9822(10) 0.111(7) Uani 0.50 1 d P
O11W O 0.9136(12) 1.3370(16) 0.9208(13) 0.156(12) Uani 0.50 1 d P
O12W O 0.6880(13) 0.7393(12) 0.8840(11) 0.105(6) Uani 0.50 1 d P
O13W O 0.0303(14) 0.7008(19) 0.6856(11) 0.160(12) Uani 0.50 1 d P
O14W O 0.2312(7) 0.7159(5) 0.6521(5) 0.103(3) Uani 1 1 d .
O15W O 0.6111(6) 0.2881(6) 0.4345(7) 0.111(3) Uani 1 1 d .
Cu1 Cu 0.36246(6) 1.12869(5) 0.61393(5) 0.0244(2) Uani 1 1 d .
Cu2 Cu 0.25575(6) 1.09439(5) 0.74219(5) 0.0244(2) Uani 1 1 d .
Cu3 Cu 0.44024(6) 1.20776(5) 0.77509(5) 0.0227(2) Uani 1 1 d .
Cu4 Cu 0.40222(6) 0.94311(5) 0.98707(5) 0.0231(2) Uani 1 1 d .
Mo1 Mo 0.65585(4) 1.16062(4) 0.86629(4) 0.02574(16) Uani 1 1 d .
Mo2 Mo 0.57724(5) 1.06389(4) 0.69617(4) 0.02819(16) Uani 1 1 d .
Mo3 Mo 0.44179(5) 0.83269(4) 0.82415(4) 0.02726(16) Uani 1 1 d .
Mo4 Mo 0.23718(4) 0.90931(4) 0.80763(4) 0.03018(17) Uani 1 1 d .
Mo5 Mo 0.66782(4) 0.96614(4) 0.85426(4) 0.02731(16) Uani 1 1 d .
Mo6 Mo 0.35522(5) 0.92931(4) 0.66407(4) 0.03152(17) Uani 1 1 d .
Mo7 Mo -0.02068(4) 1.28040(4) 0.52322(4) 0.03096(17) Uani 1 1 d .
Mo8 Mo 0.35927(5) 1.31244(4) 0.53315(4) 0.03317(18) Uani 1 1 d .
Mo9 Mo 0.32651(5) 1.49669(4) 0.59301(4) 0.03107(17) Uani 1 1 d .
Mo10 Mo 0.12080(5) 1.24738(5) 0.81769(4) 0.03574(18) Uani 1 1 d .
Mo11 Mo 0.29777(5) 1.52746(4) 0.77302(4) 0.03536(18) Uani 1 1 d .
Mo12 Mo 0.56428(5) 0.87090(4) 0.69376(4) 0.03520(18) Uani 1 1 d .
Mo13 Mo -0.04550(4) 1.31194(5) 0.70513(4) 0.03452(18) Uani 1 1 d .
Mo14 Mo 0.16963(5) 1.19453(5) 0.49698(4) 0.0407(2) Uani 1 1 d .
Mo15 Mo 0.31026(5) 1.36782(5) 0.85621(4) 0.03724(18) Uani 1 1 d .
V1 V 0.18816(8) 1.34442(7) 0.66255(7) 0.0221(3) Uani 1 1 d .
V2 V 0.44607(8) 1.03740(7) 0.84581(6) 0.0202(3) Uani 1 1 d .
V3 V 0.45483(8) 1.39513(8) 0.71869(7) 0.0282(3) Uani 1 1 d .
V4 V 0.04556(8) 1.13966(8) 0.63798(7) 0.0269(3) Uani 1 1 d .
V5 V 0.16662(17) 1.37646(15) 0.45767(14) 0.0453(5) Uani 0.64 1 d P
V6 V 0.1045(3) 1.4415(3) 0.8323(2) 0.0453(5) Uani 0.36 1 d P
O18W O 0.6096(13) 0.8038(12) 1.0128(10) 0.093(5) Uiso 0.50 1 d P
O16W O 0.1329(11) 0.9156(11) 1.0026(9) 0.082(5) Uiso 0.50 1 d P
O17W O 0.2224(13) 1.1001(12) 0.9485(11) 0.102(6) Uiso 0.50 1 d P
O19W O -0.059(2) -0.1216(19) 0.8188(17) 0.070(8) Uiso 0.25 1 d P
O20W O 0.6329(17) 0.5581(17) 0.7224(15) 0.144(9) Uiso 0.50 1 d P
O18B O 0.689(2) 0.8451(19) 1.0317(17) 0.067(8) Uiso 0.25 1 d P
O21W O 0.181(2) 1.370(2) 1.0345(19) 0.082(9) Uiso 0.25 1 d P
O20B O 0.662(2) 0.587(2) 0.838(2) 0.096(11) Uiso 0.25 1 d P
O22W O 0.809(2) 0.7741(19) 0.7082(17) 0.178(11) Uiso 0.50 1 d P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Mo5 O1 Mo3 155.1(3) . .
Mo5 O1 Mo12 103.0(2) . .
Mo3 O1 Mo12 101.9(2) . .
Mo12 O2 Mo3 104.9(2) . .
Mo12 O2 Mo6 104.9(2) . .
Mo3 O2 Mo6 112.2(2) . .
Mo6 O3 Mo2 150.1(3) . .
Mo6 O3 Mo12 104.6(2) . .
Mo2 O3 Mo12 105.3(2) . .
Mo1 O5 Cu4 142.7(3) 2_677 .
Mo3 O6 Cu4 139.5(3) . .
Mo1 O7 Cu3 143.2(3) . .
V2 O8 Mo1 125.7(2) . .
V2 O8 Mo5 118.2(2) . .
Mo1 O8 Mo5 93.37(17) . .
V2 O8 Mo2 120.1(2) . .
Mo1 O8 Mo2 92.65(17) . .
Mo5 O8 Mo2 100.51(16) . .
V2 O9 Cu3 123.1(3) . .
V2 O9 Cu2 118.3(3) . .
Cu3 O9 Cu2 92.72(19) . .
Mo4 O10 Cu2 142.8(3) . .
V2 O11 Cu4 128.4(3) . .
V2 O11 Cu4 118.8(2) . 2_677
Cu4 O11 Cu4 98.68(19) . 2_677
V2 O12 Mo4 126.1(2) . .
V2 O12 Mo3 116.4(2) . .
Mo4 O12 Mo3 92.79(18) . .
V2 O12 Mo6 121.8(2) . .
Mo4 O12 Mo6 92.62(17) . .
Mo3 O12 Mo6 100.52(17) . .
Mo5 O14 Cu4 135.8(3) . 2_677
V3 O15 Cu3 140.4(3) . .
V3 O16 Mo15 138.7(3) . .
V3 O16 Mo11 117.4(3) . .
Mo15 O16 Mo11 100.6(2) . .
V3 O17 Mo8 138.9(3) . .
V3 O17 Mo9 116.8(3) . .
Mo8 O17 Mo9 102.1(2) . .
V5 O18 Mo9 136.7(3) . .
V5 O18 Mo8 110.1(3) . .
Mo9 O18 Mo8 110.2(2) . .
V4 O20 Mo14 137.4(3) . .
V4 O20 Mo7 117.2(2) . .
Mo14 O20 Mo7 103.0(2) . .
V4 O21 Mo10 137.5(3) . .
V4 O21 Mo13 117.7(3) . .
Mo10 O21 Mo13 101.6(2) . .
Mo11 O22 V6 134.5(3) . .
Mo11 O22 Mo15 110.5(3) . .
V6 O22 Mo15 112.8(3) . .
Mo10 O23 Cu2 148.9(3) . .
V1 O24 Mo9 129.9(3) . .
V1 O24 Mo11 129.0(3) . .
Mo9 O24 Mo11 91.99(18) . .
V1 O25 Mo10 129.6(3) . .
V1 O25 Mo15 129.5(3) . .
Mo10 O25 Mo15 90.26(18) . .
Mo15 O26 Cu3 146.2(3) . .
Mo8 O27 Cu1 137.7(3) . .
Mo5 O29 Mo1 115.9(2) . .
Mo3 O30 Mo4 117.2(3) . .
V4 O31 Cu2 139.8(3) . .
Mo14 O32 Cu1 142.0(3) . .
Mo14 O33 Mo8 121.4(3) . .
Mo4 O35 Cu4 135.9(3) . .
Mo12 O36 Mo2 104.8(2) . .
Mo12 O36 Mo5 103.8(2) . .
Mo2 O36 Mo5 111.3(2) . .
V1 O37 Mo13 128.9(3) . .
V1 O37 Mo7 130.2(3) . .
Mo13 O37 Mo7 92.07(18) . .
V1 O38 Mo8 132.9(3) . .
V1 O38 Mo14 131.7(3) . .
Mo8 O38 Mo14 87.84(17) . .
Mo7 O40 Mo13 121.0(3) . .
Mo10 O41 Mo15 120.9(3) . .
V5 O42 Mo7 136.0(3) . .
V5 O42 Mo14 109.8(2) . .
Mo7 O42 Mo14 110.6(2) . .
Mo13 O43 V6 132.7(3) . .
Mo13 O43 Mo10 111.4(3) . .
V6 O43 Mo10 113.3(3) . .
Mo2 O45 Mo1 118.0(2) . .
Mo11 O49 Mo9 120.1(3) . .
Mo6 O54 Cu2 132.3(3) . .
Mo6 O54 Cu1 131.7(3) . .
Cu2 O54 Cu1 92.3(2) . .
Mo2 O55 Cu1 133.7(3) . .
Mo2 O55 Cu3 130.0(3) . .
Cu1 O55 Cu3 92.7(2) . .
Mo6 O66 Mo4 116.8(3) . .
Cu1 O68 Cu2 103.0(2) . .
Cu1 O68 Cu3 103.9(2) . .
Cu2 O68 Cu3 106.3(2) . .
O68 Cu1 O61 173.1(2) . .
O68 Cu1 O32 96.30(19) . .
O61 Cu1 O32 88.6(2) . .
O68 Cu1 O55 81.34(19) . .
O61 Cu1 O55 93.8(2) . .
O32 Cu1 O55 177.6(2) . .
O68 Cu1 O27 95.20(19) . .
O61 Cu1 O27 89.9(2) . .
O32 Cu1 O27 87.1(2) . .
O55 Cu1 O27 92.7(2) . .
O68 Cu1 O54 79.5(2) . .
O61 Cu1 O54 95.3(3) . .
O32 Cu1 O54 95.1(2) . .
O55 Cu1 O54 84.8(2) . .
O27 Cu1 O54 174.40(19) . .
O10 Cu2 O68 171.1(2) . .
O10 Cu2 O23 92.0(2) . .
O68 Cu2 O23 93.5(2) . .
O10 Cu2 O54 92.3(2) . .
O68 Cu2 O54 82.8(2) . .
O23 Cu2 O54 173.6(2) . .
O10 Cu2 O31 91.2(2) . .
O68 Cu2 O31 96.2(2) . .
O23 Cu2 O31 86.0(2) . .
O54 Cu2 O31 89.2(2) . .
O10 Cu2 O9 94.4(2) . .
O68 Cu2 O9 78.51(19) . .
O23 Cu2 O9 91.01(19) . .
O54 Cu2 O9 93.35(19) . .
O31 Cu2 O9 173.8(2) . .
O7 Cu3 O68 169.9(2) . .
O7 Cu3 O15 88.7(2) . .
O68 Cu3 O15 96.9(2) . .
O7 Cu3 O9 92.8(2) . .
O68 Cu3 O9 82.5(2) . .
O15 Cu3 O9 174.3(2) . .
O7 Cu3 O26 97.1(2) . .
O68 Cu3 O26 91.57(19) . .
O15 Cu3 O26 87.1(2) . .
O9 Cu3 O26 87.3(2) . .
O7 Cu3 O55 91.7(2) . .
O68 Cu3 O55 79.7(2) . .
O15 Cu3 O55 92.0(2) . .
O9 Cu3 O55 93.4(2) . .
O26 Cu3 O55 171.1(2) . .
O6 Cu4 O14 177.5(2) . 2_677
O6 Cu4 O5 90.2(2) . .
O14 Cu4 O5 92.1(2) 2_677 .
O6 Cu4 O11 90.7(2) . .
O14 Cu4 O11 86.9(2) 2_677 .
O5 Cu4 O11 175.1(2) . .
O6 Cu4 O35 88.1(2) . .
O14 Cu4 O35 92.9(2) 2_677 .
O5 Cu4 O35 92.9(2) . .
O11 Cu4 O35 92.0(2) . .
O6 Cu4 O11 91.01(19) . 2_677
O14 Cu4 O11 87.69(19) 2_677 2_677
O5 Cu4 O11 93.9(2) . 2_677
O11 Cu4 O11 81.32(19) . 2_677
O35 Cu4 O11 173.20(18) . 2_677
O46 Mo1 O5 104.1(3) . 2_677
O46 Mo1 O7 104.5(3) . .
O5 Mo1 O7 102.8(2) 2_677 .
O46 Mo1 O29 95.3(3) . .
O5 Mo1 O29 87.6(2) 2_677 .
O7 Mo1 O29 154.4(2) . .
O46 Mo1 O45 94.0(3) . .
O5 Mo1 O45 155.2(2) 2_677 .
O7 Mo1 O45 88.7(2) . .
O29 Mo1 O45 73.7(2) . .
O46 Mo1 O8 163.4(2) . .
O5 Mo1 O8 86.6(2) 2_677 .
O7 Mo1 O8 85.1(2) . .
O29 Mo1 O8 72.10(19) . .
O45 Mo1 O8 72.40(19) . .
O65 Mo2 O55 104.0(3) . .
O65 Mo2 O45 104.1(3) . .
O55 Mo2 O45 98.5(3) . .
O65 Mo2 O3 100.3(3) . .
O55 Mo2 O3 90.3(2) . .
O45 Mo2 O3 151.1(2) . .
O65 Mo2 O36 94.2(2) . .
O55 Mo2 O36 157.3(2) . .
O45 Mo2 O36 89.8(2) . .
O3 Mo2 O36 73.0(2) . .
O65 Mo2 O8 166.3(2) . .
O55 Mo2 O8 89.7(2) . .
O45 Mo2 O8 74.4(2) . .
O3 Mo2 O8 78.22(18) . .
O36 Mo2 O8 72.27(17) . .
O4 Mo3 O6 103.9(3) . .
O4 Mo3 O30 103.0(3) . .
O6 Mo3 O30 98.5(2) . .
O4 Mo3 O1 100.5(2) . .
O6 Mo3 O1 91.6(2) . .
O30 Mo3 O1 151.3(2) . .
O4 Mo3 O2 94.1(2) . .
O6 Mo3 O2 159.3(2) . .
O30 Mo3 O2 87.2(2) . .
O1 Mo3 O2 74.9(2) . .
O4 Mo3 O12 166.5(2) . .
O6 Mo3 O12 89.6(2) . .
O30 Mo3 O12 74.6(2) . .
O1 Mo3 O12 78.69(18) . .
O2 Mo3 O12 72.64(18) . .
O62 Mo4 O35 105.0(3) . .
O62 Mo4 O10 103.5(3) . .
O35 Mo4 O10 102.7(3) . .
O62 Mo4 O30 95.7(3) . .
O35 Mo4 O30 90.6(2) . .
O10 Mo4 O30 152.7(2) . .
O62 Mo4 O66 92.3(3) . .
O35 Mo4 O66 157.7(2) . .
O10 Mo4 O66 86.4(2) . .
O30 Mo4 O66 73.4(2) . .
O62 Mo4 O12 162.0(3) . .
O35 Mo4 O12 88.3(2) . .
O10 Mo4 O12 84.9(2) . .
O30 Mo4 O12 71.61(19) . .
O66 Mo4 O12 72.09(19) . .
O34 Mo5 O14 104.0(3) . .
O34 Mo5 O29 102.7(3) . .
O14 Mo5 O29 97.5(2) . .
O34 Mo5 O1 101.7(3) . .
O14 Mo5 O1 93.1(2) . .
O29 Mo5 O1 150.1(2) . .
O34 Mo5 O36 92.9(2) . .
O14 Mo5 O36 161.1(2) . .
O29 Mo5 O36 86.7(2) . .
O1 Mo5 O36 75.0(2) . .
O34 Mo5 O8 165.6(2) . .
O14 Mo5 O8 90.41(19) . .
O29 Mo5 O8 74.54(19) . .
O1 Mo5 O8 77.55(19) . .
O36 Mo5 O8 72.90(17) . .
O64 Mo6 O54 105.2(3) . .
O64 Mo6 O66 104.0(3) . .
O54 Mo6 O66 98.8(3) . .
O64 Mo6 O3 99.7(3) . .
O54 Mo6 O3 90.8(2) . .
O66 Mo6 O3 151.0(2) . .
O64 Mo6 O2 95.1(3) . .
O54 Mo6 O2 155.9(2) . .
O66 Mo6 O2 88.7(2) . .
O3 Mo6 O2 72.7(2) . .
O64 Mo6 O12 166.6(2) . .
O54 Mo6 O12 88.0(2) . .
O66 Mo6 O12 75.6(2) . .
O3 Mo6 O12 77.46(18) . .
O2 Mo6 O12 71.58(17) . .
O50 Mo7 O56 104.1(3) . .
O50 Mo7 O42 99.3(3) . .
O56 Mo7 O42 101.5(3) . .
O50 Mo7 O40 101.6(3) . .
O56 Mo7 O40 98.1(3) . .
O42 Mo7 O40 146.8(2) . .
O50 Mo7 O20 161.7(2) . .
O56 Mo7 O20 93.4(2) . .
O42 Mo7 O20 71.8(2) . .
O40 Mo7 O20 80.5(2) . .
O50 Mo7 O37 86.4(2) . .
O56 Mo7 O37 166.4(3) . .
O42 Mo7 O37 85.0(2) . .
O40 Mo7 O37 71.0(2) . .
O20 Mo7 O37 77.07(18) . .
O52 Mo8 O27 103.6(3) . .
O52 Mo8 O33 101.9(3) . .
O27 Mo8 O33 100.9(2) . .
O52 Mo8 O17 100.3(3) . .
O27 Mo8 O17 93.6(2) . .
O33 Mo8 O17 149.7(2) . .
O52 Mo8 O18 94.7(2) . .
O27 Mo8 O18 159.5(2) . .
O33 Mo8 O18 83.9(2) . .
O17 Mo8 O18 73.94(19) . .
O52 Mo8 O38 169.9(2) . .
O27 Mo8 O38 85.9(2) . .
O33 Mo8 O38 72.5(2) . .
O17 Mo8 O38 82.3(2) . .
O18 Mo8 O38 76.48(18) . .
O28 Mo9 O39 103.7(3) . .
O28 Mo9 O18 99.2(2) . .
O39 Mo9 O18 100.7(3) . .
O28 Mo9 O49 101.3(3) . .
O39 Mo9 O49 97.7(3) . .
O18 Mo9 O49 148.2(2) . .
O28 Mo9 O17 162.9(2) . .
O39 Mo9 O17 92.7(2) . .
O18 Mo9 O17 72.62(19) . .
O49 Mo9 O17 80.9(2) . .
O28 Mo9 O24 86.8(2) . .
O39 Mo9 O24 166.7(2) . .
O18 Mo9 O24 85.3(2) . .
O49 Mo9 O24 72.0(2) . .
O17 Mo9 O24 77.69(18) . .
O44 Mo10 O23 103.8(3) . .
O44 Mo10 O41 99.1(3) . .
O23 Mo10 O41 101.6(2) . .
O44 Mo10 O21 99.7(3) . .
O23 Mo10 O21 92.6(2) . .
O41 Mo10 O21 152.9(2) . .
O44 Mo10 O43 93.6(3) . .
O23 Mo10 O43 159.4(2) . .
O41 Mo10 O43 86.1(2) . .
O21 Mo10 O43 73.4(2) . .
O44 Mo10 O25 168.7(3) . .
O23 Mo10 O25 86.0(2) . .
O41 Mo10 O25 73.2(2) . .
O21 Mo10 O25 85.1(2) . .
O43 Mo10 O25 77.85(19) . .
O59 Mo11 O60 104.7(3) . .
O59 Mo11 O22 101.4(3) . .
O60 Mo11 O22 100.6(3) . .
O59 Mo11 O49 98.0(3) . .
O60 Mo11 O49 100.9(3) . .
O22 Mo11 O49 146.2(2) . .
O59 Mo11 O16 91.0(3) . .
O60 Mo11 O16 164.0(3) . .
O22 Mo11 O16 72.9(2) . .
O49 Mo11 O16 79.4(2) . .
O59 Mo11 O24 165.8(3) . .
O60 Mo11 O24 87.0(3) . .
O22 Mo11 O24 83.8(2) . .
O49 Mo11 O24 71.6(2) . .
O16 Mo11 O24 77.87(18) . .
O67 Mo12 O63 102.7(3) . .
O67 Mo12 O2 103.7(3) . .
O63 Mo12 O2 103.3(3) . .
O67 Mo12 O36 103.7(3) . .
O63 Mo12 O36 103.6(3) . .
O2 Mo12 O36 136.0(2) . .
O67 Mo12 O3 88.2(3) . .
O63 Mo12 O3 169.2(2) . .
O2 Mo12 O3 73.5(2) . .
O36 Mo12 O3 73.6(2) . .
O67 Mo12 O1 172.8(3) . .
O63 Mo12 O1 84.5(2) . .
O2 Mo12 O1 74.4(2) . .
O36 Mo12 O1 74.1(2) . .
O3 Mo12 O1 84.63(18) . .
O51 Mo13 O58 104.2(3) . .
O51 Mo13 O43 100.8(3) . .
O58 Mo13 O43 102.1(3) . .
O51 Mo13 O40 101.2(3) . .
O58 Mo13 O40 96.2(3) . .
O43 Mo13 O40 146.8(2) . .
O51 Mo13 O21 164.7(2) . .
O58 Mo13 O21 90.8(2) . .
O43 Mo13 O21 72.5(2) . .
O40 Mo13 O21 79.9(2) . .
O51 Mo13 O37 87.7(2) . .
O58 Mo13 O37 164.6(3) . .
O43 Mo13 O37 84.8(2) . .
O40 Mo13 O37 71.6(2) . .
O21 Mo13 O37 78.11(18) . .
O53 Mo14 O32 103.6(3) . .
O53 Mo14 O33 102.3(3) . .
O32 Mo14 O33 99.9(2) . .
O53 Mo14 O20 98.8(3) . .
O32 Mo14 O20 94.8(2) . .
O33 Mo14 O20 150.6(2) . .
O53 Mo14 O42 95.6(3) . .
O32 Mo14 O42 159.1(2) . .
O33 Mo14 O42 83.9(2) . .
O20 Mo14 O42 73.7(2) . .
O53 Mo14 O38 171.8(3) . .
O32 Mo14 O38 83.7(2) . .
O33 Mo14 O38 72.6(2) . .
O20 Mo14 O38 83.9(2) . .
O42 Mo14 O38 77.78(19) . .
O48 Mo15 O26 103.7(3) . .
O48 Mo15 O41 99.0(3) . .
O26 Mo15 O41 100.8(3) . .
O48 Mo15 O16 101.0(3) . .
O26 Mo15 O16 91.7(2) . .
O41 Mo15 O16 153.1(2) . .
O48 Mo15 O22 93.8(3) . .
O26 Mo15 O22 159.7(2) . .
O41 Mo15 O22 86.4(2) . .
O16 Mo15 O22 74.5(2) . .
O48 Mo15 O25 168.0(3) . .
O26 Mo15 O25 86.6(2) . .
O41 Mo15 O25 72.6(2) . .
O16 Mo15 O25 84.7(2) . .
O22 Mo15 O25 77.4(2) . .
O38 V1 O24 109.0(3) . .
O38 V1 O37 109.4(3) . .
O24 V1 O37 109.6(3) . .
O38 V1 O25 106.9(3) . .
O24 V1 O25 110.9(3) . .
O37 V1 O25 111.0(3) . .
O11 V2 O9 108.3(2) . .
O11 V2 O12 107.6(3) . .
O9 V2 O12 109.0(2) . .
O11 V2 O8 109.8(2) . .
O9 V2 O8 107.6(2) . .
O12 V2 O8 114.3(2) . .
O47 V3 O15 105.3(3) . .
O47 V3 O17 110.6(3) . .
O15 V3 O17 107.0(3) . .
O47 V3 O16 112.4(3) . .
O15 V3 O16 106.2(3) . .
O17 V3 O16 114.6(2) . .
O31 V4 O57 105.5(3) . .
O31 V4 O21 105.8(3) . .
O57 V4 O21 111.3(3) . .
O31 V4 O20 106.9(3) . .
O57 V4 O20 112.3(3) . .
O21 V4 O20 114.2(3) . .
O69 V5 O70 100.0(7) . .
O69 V5 O18 106.6(4) . .
O70 V5 O18 110.5(6) . .
O69 V5 O42 105.5(4) . .
O70 V5 O42 112.4(6) . .
O18 V5 O42 119.7(3) . .
O72 V6 O71 89.8(12) . .
O72 V6 O22 109.0(7) . .
O71 V6 O22 114.0(8) . .
O72 V6 O43 112.9(7) . .
O71 V6 O43 111.0(9) . .
O22 V6 O43 117.0(3) . .
O18W O18B O17W 175(3) . 2_677
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
O1 Mo5 1.970(5) .
O1 Mo3 1.985(5) .
O1 Mo12 2.245(5) .
O2 Mo12 1.948(6) .
O2 Mo3 2.197(5) .
O2 Mo6 2.199(5) .
O3 Mo6 1.973(5) .
O3 Mo2 1.985(6) .
O3 Mo12 2.183(5) .
O4 Mo3 1.677(5) .
O5 Mo1 1.775(5) 2_677
O5 Cu4 1.988(5) .
O6 Mo3 1.756(5) .
O6 Cu4 1.956(5) .
O7 Mo1 1.777(5) .
O7 Cu3 1.973(5) .
O8 V2 1.772(5) .
O8 Mo1 2.253(5) .
O8 Mo5 2.350(4) .
O8 Mo2 2.394(5) .
O9 V2 1.680(5) .
O9 Cu3 2.119(5) .
O9 Cu2 2.285(5) .
O10 Mo4 1.794(5) .
O10 Cu2 1.946(5) .
O11 V2 1.674(5) .
O11 Cu4 2.017(5) .
O11 Cu4 2.358(5) 2_677
O12 V2 1.754(5) .
O12 Mo4 2.284(5) .
O12 Mo3 2.347(5) .
O12 Mo6 2.399(5) .
O14 Mo5 1.761(5) .
O14 Cu4 1.963(5) 2_677
O15 V3 1.660(5) .
O15 Cu3 2.065(6) .
O16 V3 1.815(5) .
O16 Mo15 2.002(5) .
O16 Mo11 2.282(5) .
O17 V3 1.807(5) .
O17 Mo8 2.009(5) .
O17 Mo9 2.258(5) .
O18 V5 1.882(5) .
O18 Mo9 1.920(5) .
O18 Mo8 2.127(5) .
O20 V4 1.825(5) .
O20 Mo14 1.983(5) .
O20 Mo7 2.252(5) .
O21 V4 1.823(5) .
O21 Mo10 2.006(5) .
O21 Mo13 2.254(5) .
O22 Mo11 1.892(6) .
O22 V6 1.898(7) .
O22 Mo15 2.121(6) .
O23 Mo10 1.732(5) .
O23 Cu2 2.064(5) .
O24 V1 1.723(5) .
O24 Mo9 2.327(5) .
O24 Mo11 2.348(5) .
O25 V1 1.733(5) .
O25 Mo10 2.326(5) .
O25 Mo15 2.349(5) .
O26 Mo15 1.733(5) .
O26 Cu3 2.172(6) .
O27 Mo8 1.718(5) .
O27 Cu1 2.190(5) .
O28 Mo9 1.711(5) .
O29 Mo5 1.840(6) .
O29 Mo1 2.109(5) .
O30 Mo3 1.832(5) .
O30 Mo4 2.094(5) .
O31 V4 1.631(5) .
O31 Cu2 2.173(6) .
O32 Mo14 1.715(5) .
O32 Cu1 2.121(5) .
O33 Mo14 1.878(5) .
O33 Mo8 1.896(5) .
O34 Mo5 1.716(5) .
O35 Mo4 1.736(5) .
O35 Cu4 2.312(6) .
O36 Mo12 1.978(6) .
O36 Mo2 2.203(5) .
O36 Mo5 2.216(5) .
O37 V1 1.721(5) .
O37 Mo13 2.326(5) .
O37 Mo7 2.372(5) .
O38 V1 1.676(5) .
O38 Mo8 2.368(5) .
O38 Mo14 2.376(5) .
O39 Mo9 1.711(5) .
O40 Mo7 1.930(5) .
O40 Mo13 1.955(6) .
O41 Mo10 1.902(6) .
O41 Mo15 1.906(6) .
O42 V5 1.916(6) .
O42 Mo7 1.919(5) .
O42 Mo14 2.116(5) .
O43 Mo13 1.883(5) .
O43 V6 1.896(7) .
O43 Mo10 2.113(5) .
O44 Mo10 1.680(6) .
O45 Mo2 1.806(6) .
O45 Mo1 2.113(5) .
O46 Mo1 1.720(6) .
O47 V3 1.627(6) .
O48 Mo15 1.693(6) .
O49 Mo11 1.938(5) .
O49 Mo9 1.943(5) .
O50 Mo7 1.696(6) .
O51 Mo13 1.704(6) .
O52 Mo8 1.665(5) .
O53 Mo14 1.674(6) .
O54 Mo6 1.784(5) .
O54 Cu2 2.070(5) .
O54 Cu1 2.222(6) .
O55 Mo2 1.782(5) .
O55 Cu1 2.137(6) .
O55 Cu3 2.178(5) .
O56 Mo7 1.707(6) .
O57 V4 1.641(6) .
O58 Mo13 1.716(6) .
O59 Mo11 1.710(6) .
O60 Mo11 1.709(6) .
O61 Cu1 1.987(6) .
O62 Mo4 1.705(6) .
O63 Mo12 1.705(6) .
O64 Mo6 1.702(6) .
O65 Mo2 1.706(5) .
O66 Mo6 1.808(6) .
O66 Mo4 2.164(6) .
O67 Mo12 1.707(6) .
O68 Cu1 1.968(5) .
O68 Cu2 1.989(5) .
O68 Cu3 1.997(5) .
O69 V5 1.511(9) .
O70 V5 1.620(14) .
O71 V6 1.58(2) .
O72 V6 1.515(18) .
O2W O20W 1.80(3) .
Cu4 O14 1.963(5) 2_677
Cu4 O11 2.358(5) 2_677
Mo1 O5 1.775(5) 2_677
O18W O18B 1.31(3) .
O17W O18B 1.54(4) 2_677
O18B O17W 1.54(4) 2_677
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.071 0.333 0.119 166 22 ' '
2 -0.072 0.666 0.881 166 22 ' '
3 0.469 0.678 0.966 10 3 ' '
4 0.531 0.322 0.034 10 3 ' '
